Surface Finishing Technology Hydrogen Embrittlement
All components made from steel which are subject to chemical or
The following points should be considered when specifying electroplated
electro-chemical treatments in the course of the coating process
finishes on higher tensile parts:
may absorb hydrogen which is evolved during these processes. This absorbed hydrogen could cause premature failure if the component is
Susceptible parts subject to an embrittling process can never be
made from high tensile steel. We should like to remind customers of the
guaranteed to be completely free from embrittlement, even after
risk of hydrogen embrittlement of parts made from high tensile steel and
extensive baking treatments (ref. ISO 4042; BS 7371 Pt.1).
that baking treatments cannot be guaranteed to prevent all hydrogen
embrittlement. Parts are usually considered to be at risk if they have a
The removal of phosphate from higher tensile parts before hardening heat treatment can reduce the risk of embrittlement
tensile strength equal to or greater than 1050 MPa, 1000 N/mm or 65
(mandatory requirement for 12.9 grade fasteners and above).
tons/sq.in. (T class imperial fasteners and above) or have a hardness greater than 320vickers (HV). (10.9 fasteners and above).
The risk of embrittlement increases with increasing tensile strength. and with the use of higher tensile loads.
Baking parts after coating will minimise the risk of failure, but this
process can never be assumed to be 100% effective.
Changing the coating already applied to fasteners, i.e. stripping and replating, can be a high risk area that we will only undertake under certain circumstances. Discussion with the customer and
Embrittled parts usually fail when in use under stresses well below their
end user is essential.
normal failure level and most embrittlement failures occur in a relatively short time after assembly, between a few minutes and up to eight weeks.
The use of non-embrittling processes such as mechanical plating, zinc flake or organic coating, should be considered for susceptible
Although many studies have taken place into hydrogen embrittlement
failures, the exact reasons for the phenomenon have not been explained.
There is a slight possibility that work mechanically plated and used within six hours of processing can exhibit early failure due
The higher the tensile strength, the more susceptible to embrittlement a
to transient embrittlement. This transient embrittlement dissipates
component becomes, but also the presence of phosphate (not removed
completely after six hours. If use is envisaged within six hours of
prior to heat treatment) and other elements can alter this susceptibility
processing, please discuss with us.
Due to these risks and the availability of risk free processes, it is
If hydrogen embrittlement is identified as a risk, the use of a non-
not our policy to electroplate 12.9 grade fasteners and above, and
embrittling cleaning and coating process such as zinc flake or
we would encourage you - our customer - to follow this course of
mechanical zinc should be considered.
action also. If it is still required that we should electroplate 12.9
grade and above, we will do so only provided we receive written acknowledgement that our customers understand and accept
Most electroplating specifications give procedures to minimise the risk
these risks. We would also point out that most OEM’s forbid the
of embrittlement of high tensile parts. See the table below:
electroplating of fasteners of grade 12.9 and above.
USUAL REQUIREMENTS TO LIMIT HYDROGEN EMBRITTLEMENT Parts heat treated or cold worked to a surface hardness of
It should be noted that de-embrittlement by the baking process becomes less efficient when
TENSILE STRENGTH OF PART
high thicknesses of metals are applied due to the
390HV and above
porosity of the deposit becoming significantly
Fasteners property classes
12.9 and above
less with higher thicknesses. Some specifications
Process Requirements Clean parts to remove phosphate coating prior to hardening heat treatment
Use special wet cleaning methods
Use non-electroplated coatings
Advised 4-12 hours
It is our general policy to bake work within 1 hour of processing to minimise the risk of embrittlement.
Only allowed under special circumstances Very strongly advised Mandatory with Auto Manufacturers 24 hours (or longer)
Information presented in this data sheet is considered reliable, but conditions and methods of use, which are beyond our control, may modify results. Before these product are used, the user should confirm their suitability. We cannot accept liability for any loss, injury or damage which may result from its use. We do not warranty the accuracy or completeness of any such information whether orally or in writing. We reserve the right at anytime and without notice to update or improve products and processes and our information concerning the same.
>12µm) to be applied in two stages with a baking process after the application of 5-8 µm.
Use abrasive cleaning methods
Baking times (at 180-210°C) if electroplated
acknowledge this and expect thick coatings (e.g
Note: Phosphating can cause hydrogen embrittlement but it is generally considered that this disappears if the components are not used for 48 hours after processing otherwise a de-embrittlement baking of a minimum of 4 hours at 200oC is recommended.